Reading. Chapter 12 in DeGraef and McHenry Chapter 3i in Engler and Randle


 Bruno Payne
 2 years ago
 Views:
Transcription
1 Class 17 Xray Diffraction Chapter 1 in DeGraef and McHenry Chapter 3i in Engler and Randle Reading Chapter 6 in DeGraef and McHenry (I WILL ASSUME THAT YOU KNOW ABOUT THIS CONCEPT ALREADY! IF NOT, READ IT!) Prof. M.L. Weaver
2 Review: XRay Diffraction XRD is a powerful experimental technique used to determine the crystal structure and its lattice parameters (a, bc)and b, c, ) spacing between lattice planes (hkl Miller indices) this interplanar spacing (d) is the distance between parallel planes of atoms or ions. Diffraction is result of radiation s being scattered by a regular array of scattering centers whose spacing is about same as the of the radiation. Diffraction gratings must have spacings comparable to the wavelength of diffracted radiation. We know that atoms and ions are on the order of 0.1 nm in size, so we think of crystal structures as being diffraction gratings on a subnanometer scale. For Xrays, atoms are scattering centers (photon interaction with an orbital electron in the atom). Spacing (d hkl ) is the distance between parallel planes of atoms
3 XRD to Determine Crystal Structure & Interplanar Spacing Recall incoming Xrays diffract from crystal planes: extra distance traveled by wave Adapted from Fig. 3.37, Callister & Rethwisch 3e. is scattering (Bragg) angle Measurement of critical angle, c, allows computation of interplanar spacing (d) Xray intensity (from detector) d spacing between planes d sin c a Bragg s Law (1) d hkl cubic h k l () Combine (1)+(): c reflections must be in phase for a detectable signal i.e., for diffraction to occur, xrays scattered off adjacent crystal planes must be in phase: (Bragg s Law is not satisfied) 3
4 Recall the interplanar spacings (d hkl ) for the 7 crystal systems As crystal symmetry decreases, the number of peaks observed increases: Cubic crystals, highest symmetry, fewest peaks. Triclinic crystals, lowest symmetry, large number of peaks. 4
5 Geometry of XRD (F.Y.I) A single wavelength of xray radiation is often used to keep the number of diffraction peaks to a small workable number, since samples often consists of many small crystal grains orientated randomly. The diffracted beam intensity is monitored electronically by a mechanically driven scanning radiation detector. Collimate beam Usually graphite to focus beam like a parabolic mirror High Z to max. absorption. Removing unwanted radiation Xray Source (fixed) Bragg angle = Diffraction angle, what s measured experimentally = Counter/detector is rotated about Oaxis; is its angular position. Counter and specimen are mechanically coupled such that a rotation of the specimen through is accompanied by a rotation of the counter. This assures that the incident and reflection angles are maintained equal to one another.
6 More on Bragg s Law Bragg s Law is a necessary but insufficient condition for diffraction. It only defines the diffraction condition for primitive unit cells, e.g. P cubic, P tetragonal, etc., where atoms are only at unit cell corners. Crystal structures with nonprimitive unit cells have atoms at additional lattice (basis) sites. These extra scattering centers can cause outofphase scattering to occur at certain Bragg angles. The net result is that some of the diffraction predicted by Bragg s Law (eq. 1) does not occur, i.e. certain sets of planes do not exist (forbidden reflections). Selection (or Reflection) rules: Bravais Lattice Example Compounds Allowed Reflections Forbidden Reflections Primitive Cubic Simple Cubic (Po) Any h,k,l None BodyCentered Cubic BodyCentered Cubic metal h+k+l even h+k+l odd FaceCentered Cubic FaceCentered Cubic metal h,k,l all odd or all even h,k,l mixed odd or even FaceCentered Cubic NaClrocksalt, ZnSzincblende h,k,l all odd or all even h,k,l mixed odd or even FaceCentered Cubic Si, Ge Diamond cubic As FCC, but if all even hkl h,k,l mixed odd or even and h+k+l 4n, then and if all even and absent (n is integer) h+k+l 4n Primitive Hexagonal Hexagonal closed packed metal All other cases h+k=3n, l odd These rules are calculated based on atomic scattering factors and structure factors, which we will discuss next class and next week (you will also see on final exam). 6
7 Selection Rules for Cubic Crystals P I F a a d hkl S (hkl) S (hkl) S (hkl) h k l S where S is reflection or line #, e.g. (100) is 1 st order reflection and (00) is 4 th order reflection As we will determine later when we calculate the structure factors, these selection rules also hold 9 1, for other Bravais lattices, e.g Itetragonal, Forthorhombic, etc Odd+even Odd+even All odd All even Odd+even Odd+even All even Odd+even Odd+even All odd All even 7
8 Example of XRD Pattern The unit cell size and geometry may be resolved from the angular positions of the diffraction peaks. When the distance between the peak spacings are all pretty much the same () it is likely cubic. The arrangement of atoms within the unit cell is associated with the relative intensities of these peaks c z c z (110) (00) (11) c z lative) In ntensity (re a b x Diffraction pattern for polycrystalline y iron (BCC) y (110) a x (00) b y dspacing decreases according to Bragg s Law a x (11) b y Diffraction angle h+k+l even are only allowed according to previously shown selection rules for BCC. 8
9 Review of Systematic Absences in the Diffraction Patterns of 4 Cubic Structures =S= When indexing XRD data for your material always try cubic first (least amount of diffracting planes since most symmetric lattice parameters). 9
10 Bragg s Law (1): d sin c a d hkl h k l Combined (1) and (): n sin or a h k l XRay Diffraction for Tetragonal, Hexagonal and Orthorhombic o ccrystals s (1) () Plane spacing for cubic crystals Plane spacings for: sin If crystal is tetragonal with a=a c then (1) and (4) become: ( h k l ) 4a (3) sin h k l (7) 4a 4c For a particular incident xray wavelength and cubic crystal of unit cell size a, this equation predicts all possible If crystal is hexagonal with a=a c then (1) and (5) become: Bragg angles at which diffraction can occur from planes sin h k hk l (hkl). (8) 3a 4c If crystal is orthorhombic with a b c then (1) and (6): Diffraction planes are determined solely by the shape and size (lattice parameters) of the unit cell. sin ( h ) ( k ) ( l ) (9) 4a 4b 4c Intensities of diffracted beams are determined by positions of the atoms within the unit cell. Thus, we must measure the intensities if we are able to obtain any information at all about atom positions. (Intensities (I) are related to Structure Factor (F); i.e.,, I is proportional p to F). We will determine that for many crystals there are particular atomic arrangements which reduce the intensities of some diffracted beams to zero, i.e. no diffracted beam at the angle () predicted by Equations (3), (7), (8), (9), etc., which means F=0. 10 (4) (5) (6)
11 The Effect of Cell Distortion (Symmetry) on XRD Patterns As the symmetry of crystal decreases more peaks are seen, e.g. cubic triclinic. Similar with cell distortion. If distort cubic I along [001] by 4% so c is now, 416Å 4.16Å get tii tetragonal. This decreases symmetry more, and shifted diffraction lines are formed (shown in the middle for tetragonal). If now stretch 8% along [010] axis with a=4.00å, b= 4.3Å, and c= 4.16Å to get orthorhombic I which lowers symmetry even more thus adding more diffraction lines (shown right). The increase in number of lines is due to the introduction of new hkl plane dspacings, caused by nonuniform distortion. Thus in cubic cell, the (00), (00) and (00) planes all have the same spacing and only one line is formed, called the (00) line. However, this line splits into two when the cell becomes tetragonal since now the (00) plane spacing differs from the other two. When the cell becomes orthorhombic, all three spacings are different and three lines are formed. Common in phase transformations, e.g. carbon steel slowly cooled get Ferrite (BCC) Cementite (orthor.), and quench from austentite (FCC) martensite (Itetragonal). In disorderorder reactions (CuAu), cubic in disordered state but becomes either tetragonal or orthorhombic (depending on temperature) when ordered
12 Example: Phase Transformations in ZrO Lowpressure forms of ZrO. Red=O Blue=Zr Property Cubic ZrO Tetragonal ZrO Monoclinic ZrO Lattice parameters (Å) a b c Temperature (K) > to 570 <1400 Coordination Zr=8; Zr=8; O 1 =4; O =4 O 1 =4; O =4 Volume (Å 3 ) Density (g/cc) Space Group Fm3m P4 /nmc P 1 /c Zr=7; O 1 =3; O =4 XRD scan of a tetragonal ZrO thin film taken from UNT s Rigaku Ultima III highresolution XRD 1
13 Monoclinic Cubic 13
Crystal Structure Determination I
Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationXray thinfilm measurement techniques
Technical articles Xray thinfilm measurement techniques II. Outofplane diffraction measurements Toru Mitsunaga* 1. Introduction A thinfilm sample is twodimensionally formed on the surface of a substrate,
More informationLMB Crystallography Course, 2013. Crystals, Symmetry and Space Groups Andrew Leslie
LMB Crystallography Course, 2013 Crystals, Symmetry and Space Groups Andrew Leslie Many of the slides were kindly provided by Erhard Hohenester (Imperial College), several other illustrations are from
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationXRay Diffraction. wavelength Electric field of light
Light is composed of electromagnetic radiation with an electric component that modulates versus time perpendicular to the direction it is travelling (the magnetic component is also perpendicular to the
More informationIntroduction to Powder XRay Diffraction History Basic Principles
Introduction to Powder XRay Diffraction History Basic Principles Folie.1 History: Wilhelm Conrad Röntgen Wilhelm Conrad Röntgen discovered 1895 the Xrays. 1901 he was honoured by the Noble prize for
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationLAUE DIFFRACTION INTRODUCTION CHARACTERISTICS X RAYS BREMSSTRAHLUNG
LAUE DIFFRACTION INTRODUCTION Xrays are electromagnetic radiations that originate outside the nucleus. There are two major processes for Xray production which are quite different and which lead to different
More informationChapter 3: Structure of Metals and Ceramics. Chapter 3: Structure of Metals and Ceramics. Learning Objective
Chapter 3: Structure of Metals and Ceramics Chapter 3: Structure of Metals and Ceramics Goals Define basic terms and give examples of each: Lattice Basis Atoms (Decorations or Motifs) Crystal Structure
More informationXray Diffraction (XRD)
Xray Diffraction (XRD) 1.0 What is Xray Diffraction 2.0 Basics of Crystallography 3.0 Production of Xrays 4.0 Applications of XRD 5.0 Instrumental Sources of Error 6.0 Conclusions Bragg s Law n l =2dsinq
More informationChapters 2 and 6 in Waseda. Lesson 8 Lattice Planes and Directions. Suggested Reading
Analytical Methods for Materials Chapters 2 and 6 in Waseda Lesson 8 Lattice Planes and Directions Suggested Reading 192 Directions and Miller Indices Draw vector and define the tail as the origin. z Determine
More informationStructure Factors 59553 78
78 Structure Factors Until now, we have only typically considered reflections arising from planes in a hypothetical lattice containing one atom in the asymmetric unit. In practice we will generally deal
More informationSolid State Device Fundamentals
Solid State Device Fundamentals ENS 345 Lecture Course by Alexander M. Zaitsev alexander.zaitsev@csi.cuny.edu Tel: 718 982 2812 Office 4N101b 1 Solids Three types of solids, classified according to atomic
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationChapter 7: Basics of Xray Diffraction
Providing Solutions To Your Diffraction Needs. Chapter 7: Basics of Xray Diffraction Scintag has prepared this section for use by customers and authorized personnel. The information contained herein is
More informationBCM 6200  Protein crystallography  I. Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS
BCM 6200  Protein crystallography  I Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS Elastic Xray Scattering From classical electrodynamics, the electric field of the electromagnetic
More informationXRAY DIFFRACTION PROCEDURES
XRAY DIFFRACTION PROCEDURES For Polycrystalline and Amorphous Materials HAROLD P. KLUG HEAD OF THE DEPARTMENT OF RESEARCH IN CHEMICAL PHYSICS LEROY E. ALEXANDER SENIOR FELLOW IN XRAY DIFFRACTION Mellon
More informationTheory of XRay Diffraction. Kingshuk Majumdar
Theory of XRay Diffraction Kingshuk Majumdar Contents Introduction to XRays Crystal Structures: Introduction to Lattices Different types of lattices Reciprocal Lattice Index Planes XRay Diffraction:
More informationXray diffraction techniques for thin films
Xray diffraction techniques for thin films Rigaku Corporation Application Laboratory Takayuki Konya 1 Today s contents (PM) Introduction Xray diffraction method OutofPlane InPlane Pole figure Reciprocal
More informationPolarization Dependence in Xray Spectroscopy and Scattering. S P Collins et al Diamond Light Source UK
Polarization Dependence in Xray Spectroscopy and Scattering S P Collins et al Diamond Light Source UK Overview of talk 1. Experimental techniques at Diamond: why we care about xray polarization 2. How
More informationPOWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS
EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort
More informationIntroduction to XRay Powder Diffraction Data Analysis
Introduction to XRay Powder Diffraction Data Analysis Center for Materials Science and Engineering at MIT http://prism.mit.edu/xray An Xray diffraction pattern is a plot of the intensity of Xrays scattered
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationCrystal Structure of High Temperature Superconductors. Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson
Crystal Structure of High Temperature Superconductors Marie Nelson East Orange Campus High School NJIT Professor: Trevor Tyson Introduction History of Superconductors Superconductors are material which
More informationEach grain is a single crystal with a specific orientation. Imperfections
Crystal Structure / Imperfections Almost all materials crystallize when they solidify; i.e., the atoms are arranged in an ordered, repeating, 3dimensional pattern. These structures are called crystals
More informationXray Diffraction and EBSD
Xray Diffraction and EBSD Jonathan Cowen Swagelok Center for the Surface Analysis of Materials Case School of Engineering Case Western Reserve University October 27, 2014 Outline Xray Diffraction (XRD)
More informationThe Crystal Structures of Solids
The Crystal Structures of Solids Crystals of pure substances can be analyzed using Xray diffraction methods to provide valuable information. The type and strength of intramolecular forces, density, molar
More information6) How wide must a narrow slit be if the first diffraction minimum occurs at ±12 with laser light of 633 nm?
Test IV Name 1) In a single slit diffraction experiment, the width of the slit is 3.1 105 m and the distance from the slit to the screen is 2.2 m. If the beam of light of wavelength 600 nm passes through
More informationThe Structure of solids.
Chapter S. The Structure of solids. After having studied this chapter, the student will be able to: 1. Distinguish between a crystal structure and an amorphous structure. 2. Describe the concept of a unit
More informationMULTIPLE CHOICE. Choose the one alternative that best completes the statement or answers the question.
Exam Name MULTIPLE CHOICE. Choose the one alternative that best completes the statement or answers the question. 1) A single slit forms a diffraction pattern, with the first minimum at an angle of 40 from
More informationWAVELENGTH OF LIGHT  DIFFRACTION GRATING
PURPOSE In this experiment we will use the diffraction grating and the spectrometer to measure wavelengths in the mercury spectrum. THEORY A diffraction grating is essentially a series of parallel equidistant
More informationChem 106 Thursday Feb. 3, 2011
Chem 106 Thursday Feb. 3, 2011 Chapter 13: The Chemistry of Solids Phase Diagrams  (no BornHaber cycle) 2/3/2011 1 Approx surface area (Å 2 ) 253 258 Which C 5 H 12 alkane do you think has the highest
More informationUsing light scattering method to find The surface tension of water
Experiment (8) Using light scattering method to find The surface tension of water The aim of work: The goals of this experiment are to confirm the relationship between angular frequency and wave vector
More informationTwinning and absolute structure. Bill Clegg Newcastle University, UK. SHELX Workshop Denver 2016
Twinning and absolute structure Bill Clegg Newcastle University, UK SHELX Workshop Denver 2016 Outline Twinning Definition, characterisation, illustration Classification: different types of twin Recognition:
More informationQuick Guide for Data Collection on the NIU Bruker Smart CCD
Quick Guide for Data Collection on the NIU Bruker Smart CCD 1. Create a new project 2. Optically align the crystal 3. Take rotation picture 4. Collect matrix to determine unit cell 5. Refine unit cell
More informationEarth Sciences: Course Presenters
Earth Sciences: Course Presenters 625102 Geology Dr Stephen Gallagher Prof Andrew Gleadow Dr Malcolm Wallace Prof Ian Plimer Course Coordinator Room 214 Series  Lecture Topics 1. Mineralogy and Crystals
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationPHOTOELECTRIC EFFECT AND DUAL NATURE OF MATTER AND RADIATIONS
PHOTOELECTRIC EFFECT AND DUAL NATURE OF MATTER AND RADIATIONS 1. Photons 2. Photoelectric Effect 3. Experimental Setup to study Photoelectric Effect 4. Effect of Intensity, Frequency, Potential on P.E.
More informationCrystal Optics of Visible Light
Crystal Optics of Visible Light This can be a very helpful aspect of minerals in understanding the petrographic history of a rock. The manner by which light is transferred through a mineral is a means
More informationAcoustooptic modulator
1 of 3 Acoustooptic modulator F An acoustooptic modulator (AOM), also called a Bragg cell, uses the acoustooptic effect to diffract and shift the frequency of light using sound waves (usually at radiofrequency).
More informationChapter 2: Crystal Structures and Symmetry
Chapter 2: Crystal Structures and Symmetry Laue, ravais December 28, 2001 Contents 1 Lattice Types and Symmetry 3 1.1 TwoDimensional Lattices................. 3 1.2 ThreeDimensional Lattices................
More informationrotation,, axis of rotoinversion,, center of symmetry, and mirror planes can be
Crystal Symmetry The external shape of a crystal reflects the presence or absence of translationfree symmetry y elements in its unit cell. While not always immediately obvious, in most well formed crystal
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More informationLecture Outline Crystallography
Lecture Outline Crystallography Short and long range Order Poly and single crystals, anisotropy, polymorphy Allotropic and Polymorphic Transitions Lattice, Unit Cells, Basis, Packing, Density, and Crystal
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More informationUnit 12 Practice Test
Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and
More informationPowder diffraction and synchrotron radiation
Powder diffraction and synchrotron radiation Gilberto Artioli Dip. Geoscienze UNIPD CIRCe Center for Cement Materials single xl diffraction powder diffraction Ideal powder Powder averaging Textured sample
More informationCHEM 10113, Quiz 7 December 7, 2011
CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationXRay Diffraction Studies of Copper Nanopowder
XRay Diffraction Studies of Copper Nanopowder T. Theivasanthi (1) and M. Alagar (2) (1) Department of Physics, PACR Polytechnic College, Rajapalayam, India. (2) Department of Physics, Ayya Nadar Janaki
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationChapter 13 The Chemistry of Solids
Chapter 13 The Chemistry of Solids Jeffrey Mack California State University, Sacramento Metallic & Ionic Solids Crystal Lattices Regular 3D arrangements of equivalent LATTICE POINTS in space. Lattice
More informationIntroduction to microstructure
Introduction to microstructure 1.1 What is microstructure? When describing the structure of a material, we make a clear distinction between its crystal structure and its microstructure. The term crystal
More informationThis is an authordeposited version published in: http://sam.ensam.eu Handle ID:.http://hdl.handle.net/10985/10324
Science Arts & Métiers (SAM) is an open access repository that collects the work of Arts et Métiers ParisTech researchers and makes it freely available over the web where possible. This is an authordeposited
More information12. CONFOCAL MICROSCOPY. Confocal microscopy can render depthresolved slices through a 3D object by
12. CONFOCAL MICROSCOPY Confocal microscopy can render depthresolved slices through a 3D object by rejecting much of the out of focus light via a pinhole. The image is reconstructed serially, i.e. point
More informationDetermination of Molecular Structure by MOLECULAR SPECTROSCOPY
Determination of Molecular Structure by MOLEULAR SPETROSOPY hemistry 3 B.Z. Shakhashiri Fall 29 Much of what we know about molecular structure has been learned by observing and analyzing how electromagnetic
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationCOMPARISON OF TEXTURE IN COPPER AND ALUMINUM THIN FILMS DETERMINED BY XRD AND EBSD *
201 COMPARISON OF TEXTURE IN COPPER AND ALUMINUM THIN FILMS DETERMINED BY XRD AND EBSD * J. Müller 1, D. Balzar 1,2, R.H. Geiss 1, D.T. Read 1, and R.R. Keller 1 1 Materials Reliability Division, National
More informationemission of light from atoms discrete line spectra  energy levels, FranckHertz experiment
Introduction Until the early 20 th century physicists used to explain the phenomena in the physical world around them using theories such a mechanics, electromagnetism, thermodynamics and statistical physics
More informationATOMIC SPECTRA. Apparatus: Optical spectrometer, spectral tubes, power supply, incandescent lamp, bottles of dyed water, elevating jack or block.
1 ATOMIC SPECTRA Objective: To measure the wavelengths of visible light emitted by atomic hydrogen and verify the measured wavelengths against those predicted by quantum theory. To identify an unknown
More informationGlancing XRD and XRF for the Study of Texture Development in SmCo Based Films Sputtered Onto Silicon Substrates
161 162 Glancing XRD and XRF for the Study of Texture Development in SmCo Based Films Sputtered Onto Silicon Substrates F. J. Cadieu*, I. Vander, Y. Rong, and R. W. Zuneska Physics Department Queens College
More informationO6: The Diffraction Grating Spectrometer
2B30: PRACTICAL ASTROPHYSICS FORMAL REPORT: O6: The Diffraction Grating Spectrometer Adam Hill Lab partner: G. Evans Tutor: Dr. Peter Storey 1 Abstract The calibration of a diffraction grating spectrometer
More informationPrinciple of Formation of Magnetic Field of Iron
Principle of Formation of Magnetic Field of Iron Anatoli Bedritsky Abstract. This article discovers physical phenomena which occur at the formation of the magnetic field of iron and the reason of an attraction
More informationLiquids and Solids. AP Chemistry Chapter 10. 9/20/2009 Jodi Grack; Wayzata High School; images used with permission from Zumdahl
Liquids and Solids AP Chemistry Chapter 10 Liquids and Solids Gases are much easier to study because molecules move independent of each other. In liquids and solids forces between molecules become very
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More informationXRay Diffraction: A Comprehensive Explanation for Multipurpose Research
XRay Diffraction: A Comprehensive Explanation for Multipurpose Research Adree Khondker 1, Shakir Lakhani 2 1 Westdale S.S., Hamilton, ON, Canada 2 Upper Canada College, Toronto, ON, Canada Abstract: The
More informationThe SternGerlach Experiment
Chapter The SternGerlach Experiment Let us now talk about a particular property of an atom, called its magnetic dipole moment. It is simplest to first recall what an electric dipole moment is. Consider
More informationAP Chemistry A. Allan Chapter 7 Notes  Atomic Structure and Periodicity
AP Chemistry A. Allan Chapter 7 Notes  Atomic Structure and Periodicity 7.1 Electromagnetic Radiation A. Types of EM Radiation (wavelengths in meters) 101 1010 108 4 to 7x107 104 101 10 10 4 gamma
More informationXray diffraction in polymer science
Xray diffraction in polymer science 1) Identification of semicrystalline polymers and Recognition of crystalline phases (polymorphism) of polymers 2)Polymers are never 100% crystalline. XRD is a primary
More informationXRay Study of Soft and Hard Magnetic Thin Films
Copyright (C) JCPDSInternational Centre for Diffraction Data 1999 13 XRay Study of Soft and Hard Magnetic Thin Films PoWen Wang, 390 Reed St., Stormedia, Inc., Santa Clara CA. 95050 Abstract : This
More informationName: Class: Date: ID: A
Name: Class: _ Date: _ Practice Quiz 4 Multiple Choice Identify the choice that best completes the statement or answers the question. 1. What is the wavelength of the longest wavelength light that can
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationInfrared Spectroscopy: Theory
u Chapter 15 Infrared Spectroscopy: Theory An important tool of the organic chemist is Infrared Spectroscopy, or IR. IR spectra are acquired on a special instrument, called an IR spectrometer. IR is used
More informationInterference. Physics 102 Workshop #3. General Instructions
Interference Physics 102 Workshop #3 Name: Lab Partner(s): Instructor: Time of Workshop: General Instructions Workshop exercises are to be carried out in groups of three. One report per group is due by
More informationApplications of XRay Absorption Spectroscopy
Applications of XRay Absorption Spectroscopy Bruce Ravel The Naval Research Laboratory ravel@phys.washington.edu http://feff.phys.washington.edu/~ravel/ Version 0.01 5 March, 2001 Abstract This document
More informationMAG*I*CAL Reference Standard for TEM
N Norrox Scientific Ltd. MAG*I*CAL Reference Standard for TEM FRAGILE! The MAG*I*CAL calibration reference standard that you are receiving now looks like Figure A, below. If not handled carefully, it will
More informationSample Exercise 12.1 Calculating Packing Efficiency
Sample Exercise 12.1 Calculating Packing Efficiency It is not possible to pack spheres together without leaving some void spaces between the spheres. Packing efficiency is the fraction of space in a crystal
More informationXray Powder Diffraction Pattern Indexing for Pharmaceutical Applications
The published version of this manuscript may be found at the following webpage: http://www.pharmtech.com/pharmtech/peerreviewed+research/xraypowderdiffractionpatternindexingfor Phar/ArticleStandard/Article/detail/800851
More informationLaue lens for Nuclear Medicine
Laue lens for Nuclear Medicine PhD in Physics Gianfranco Paternò Ferrara, 611013 Supervisor: prof. Vincenzo Guidi Sensors and Semiconductors Lab, Department of Physics and Earth Science, University of
More informationA NATIONAL MEASUREMENT GOOD PRACTICE GUIDE. No. 52. Determination of Residual Stresses by Xray Diffraction  Issue 2
A NATIONAL MEASUREMENT GOOD PRACTICE GUIDE No. 52 Determination of Residual Stresses by Xray Diffraction  Issue 2 The DTI drives our ambition of prosperity for all by working to create the best environment
More informationStructure of Metals 110
Structure of Metals 110 Welcome to the Tooling University. This course is designed to be used in conjunction with the online version of this class. The online version can be found at http://www.toolingu.com.
More informationThe nearlyfree electron model
Handout 3 The nearlyfree electron model 3.1 Introduction Having derived Bloch s theorem we are now at a stage where we can start introducing the concept of bandstructure. When someone refers to the bandstructure
More informationCRYSTALLINE SOLIDS IN 3D
CRYSTALLINE SOLIDS IN 3D Andrew Baczewski PHY 491, October 7th, 2011 OVERVIEW First  are there any questions from the previous lecture? Today, we will answer the following questions: Why should we care
More informationDOING PHYSICS WITH MATLAB COMPUTATIONAL OPTICS RAYLEIGHSOMMERFELD DIFFRACTION INTEGRAL OF THE FIRST KIND
DOING PHYSICS WITH MATLAB COMPUTATIONAL OPTICS RAYLEIGHSOMMERFELD DIFFRACTION INTEGRAL OF THE FIRST KIND THE THREEDIMENSIONAL DISTRIBUTION OF THE RADIANT FLUX DENSITY AT THE FOCUS OF A CONVERGENCE BEAM
More informationORIENTATION CHARACTERISTICS OF THE MICROSTRUCTURE OF MATERIALS
ORIENTATION CHARACTERISTICS OF THE MICROSTRUCTURE OF MATERIALS K. Sztwiertnia Polish Academy of Sciences, Institute of Metallurgy and Materials Science, 25 Reymonta St., 30059 Krakow, Poland MMN 2009
More informationChapter 8. Low energy ion scattering study of Fe 4 N on Cu(100)
Low energy ion scattering study of 4 on Cu(1) Chapter 8. Low energy ion scattering study of 4 on Cu(1) 8.1. Introduction For a better understanding of the reconstructed 4 surfaces one would like to know
More informationThe Phenomenon of Photoelectric Emission:
The Photoelectric Effect. The Wave particle duality of light Light, like any other E.M.R (electromagnetic radiation) has got a dual nature. That is there are experiments that prove that it is made up of
More informationGRID AND PRISM SPECTROMETERS
FYSA230/2 GRID AND PRISM SPECTROMETERS 1. Introduction Electromagnetic radiation (e.g. visible light) experiences reflection, refraction, interference and diffraction phenomena when entering and passing
More informationCrystalline Structures Crystal Lattice Structures
Jewelry Home Page Crystalline Structures Crystal Lattice Structures Crystal Habit Refractive Index Crystal Forms Mohs Scale Mineral Classification Crystal Healing Extensive information on healing crystals,
More informationPHYSICS PAPER 1 (THEORY)
PHYSICS PAPER 1 (THEORY) (Three hours) (Candidates are allowed additional 15 minutes for only reading the paper. They must NOT start writing during this time.) 
More informationXray Crystallography Lectures
Xray Crystallography Lectures 1. Biological imaging by Xray diffraction. An overview. 2. Crystals. Growth, physical properties and diffraction. 3. Working in reciprocal space. Xray intensity data collection
More informationCHAPTER 7: DISLOCATIONS AND STRENGTHENING
CHAPTER 7: DISLOCATIONS AND STRENGTHENING ISSUES TO ADDRESS... Why are dislocations observed primarily in metals and alloys? Mech 221  Notes 7 1 DISLOCATION MOTION Produces plastic deformation, in crystalline
More informationNanoelectronics 09. Atsufumi Hirohata Department of Electronics. Quick Review over the Last Lecture
Nanoelectronics 09 Atsufumi Hirohata Department of Electronics 12:00 Wednesday, 4/February/2015 (P/L 006) Quick Review over the Last Lecture ( Field effect transistor (FET) ): ( Drain ) current increases
More informationA program for phase identification using diffractograms obtained from TEM structure images
INVESTIGACIÓN Revista Mexicana de Física 59 (2013) 102 106 MARCH APRIL 2013 A program for phase identification using diffractograms obtained from TEM structure images R. Galicia a, R. Herrera a,, J. L.
More information